Stainless steel acid or base, and the solution temperature. Uniform corrosion is typically easy to avoid because of extensive published corrosion data or easy to perform laboratory corrosion testing. However, stainless steels are susceptible to localized corrosion under certain conditions, which need to be recognized and avoided. Such localized corrosion is problematic for stainless steels because it is unexpected and difficult to predict. Acidic solutions can be categorized into two general categories, reducing acids such as hydrochloric acid and dilute sulfuric acid, and oxidizing acids such as nitric acid and concentrated sulfuric acid. Increasing chromium and molybdenum contents provide increasing resistance to
Martensitic stainless steel and internal clamps). Untempered martensite is low in toughness and therefore brittle. The characteristic body-centered tetragonal martensite microstructure was first observed by German microscopist Adolf Martens around 1890. In 1912, Elwood Haynes applied for a U.S. patent on a martensitic stainless steel alloy. This patent was not granted until 1919. Martensitic stainless steel can be nondestructively tested using the magnetic particle inspection method, unlike austenitic stainless steel. Also in 1912, Harry Brearley of the Brown-Firth research laboratory in Sheffield, England, while seeking a corrosion-resistant alloy for gun barrels, discovered and subsequently industrialized a martensitic stainless steel alloy. The discovery was